# superconducting gap anisotropy in monolayer fese thin film

Embed Size (px)

TRANSCRIPT

Superconducting gap anisotropy in monolayer FeSe thin film

Y. Zhang1, 2, J. J. Lee1, 3, R. G. Moore1, W. Li1, M. Yi1, 3, M. Hashimoto4, D. H. Lu4, T. P.

Devereaux1, 3, D.-H. Lee5, 6 & Z.-X. Shen1, 3, *

1Stanford Institute for Materials and Energy Sciences, SLAC National Accelerator

Laboratory, 2575 Sand Hill Road, Menlo Park, California 94025, USA

2Advanced Light Source, Lawrence Berkeley National

Laboratory, Berkeley, California 94720, USA

3Geballe Laboratory for Advanced Materials, Departments of Physics and Applied Physics,

Stanford University, Stanford, California 94305, USA

4Stanford Synchrotron Radiation Lightsource, SLAC National Accelerator Laboratory,

2575 Sand Hill Road, Menlo Park, California 94025, USA

5Department of Physics, University of California at Berkeley, Berkeley, California, 94720,

USA

94720, USA

superconductor. Superconductivity in one monolayer (1ML) FeSe thin film has

attracted great interest recently due to its intriguing interfacial properties and possibly

high superconducting transition temperature (Tc) over 77 K1-12. Here, we report high-

resolution measurements of the Fermi surface and superconducting gaps in 1ML FeSe

using angle-resolved photoemission spectroscopy (ARPES). Two ellipse-like electron

pockets are clearly resolved overlapping with each other at the Brillouin zone corner.

The superconducting gap is nodeless but moderately anisotropic, which put strong

constraints on determining the pairing symmetry. The gap maxima locate along the

major axis of ellipse, which cannot be explained by a single d-wave, extended s-wave, or

s± gap function. Four gap minima are observed at the intersection of electron pockets

suggesting the existence of either a sign change or orbital-dependent pairing in 1ML

FeSe.

For 1ML FeSe thin film grown on SrTiO3, previous angle-resolved photoemission

spectroscopy (ARPES) studies showed that the Fermi surface consists only of electron

pockets at the corner of the Brillouin zone and there are no hole pockets at the zone center as

typically found in iron-based superconductors2-4, 10. Based on such a Fermi surface topology,

several pairing symmetries have been proposed theoretically13-19: d-wave and extended s-

wave pairing symmetries, where the gaps change sign between different parts of the Fermi

surface; s-wave and s± pairing symmetries, where there is no sign change on the Fermi

surface. In early studies, the superconducting gaps were found to be nearly isotropic on the

electron pockets2, 4, however they provide insufficient information to address the critical issue

of pairing symmetry in 1ML FeSe.

Here, we study the 1ML FeSe film using high-resolution ARPES. The film is grown on Nb-

doped SrTiO3 and the Tc is around 55K as reported in ref 10. As shown in Fig. 1a, the ARPES

intensity map shows one circular-like Fermi surface at M and no Fermi surface at the zone

center (Γ). This result is consistent with previous studies2-4, 10. However, by performing high-

resolution measurements at the M point using particular photon polarizations, two ellipse-like

electron pockets are clearly resolved (Figs. 1c and 1d). According to the band calculations,

the Fermi surface consists of one ellipse electron pocket at each Brillouin zone boundary in

one-iron Brillouin zone20, 21 (Fig. 1b). When the glide-mirror symmetry of the iron-selenium

plane is considered, the unit cell doubles and the Brillouin zone folds22. As a result, the

horizontal ellipse pocket (δ1) folds onto the vertical ellipse pocket (δ2) in the two-iron

Brillouin zone (Fig. 1b). This is consistent with the observed Fermi surface topology at the M

point (Figs. 1c and 1d). The photoemission intensity of the main band δ2, is much higher than

that of the folded band δ1 at the bottom corner of the two-iron Brillouin zone.

Clear delineation of Fermi surface is important for determining the gap structure in 1ML

FeSe. Figure 2 shows the superconducting gaps associated with the δ1 and δ2 electron bands

along the Γ-M direction. Two electron bands are clearly resolved in the second derivative

images along the M-Γ direction (Fig. 2a). The orbital selectivity of different polarizations

enables us to probe different bands separately22, 23, which is crucial for measuring the

superconducting gaps in a multi-band system. By using linear vertical polarization (LV), the

δ1 and δ2 bands can be probed selectively by choosing the cut momenta at either the left or

bottom corner of the Brillouin zone (Fig. 2b). The back bendings of bands are clearly

observed attesting for the high data quality. The gap magnitude is determined by the gap

fitting of symmetrized EDCs at the relevant kF’s (Figs. 2c and 2d), i.e., the gap minima of the

corresponding band dispersions (Fig. 2a). The superconducting gap is ~10 meV for the δ1

band and ~13 meV for the δ2 band.

The multi-gap behavior on δ1 and δ2 suggests that the superconducting gap is anisotropic. By

choosing different experimental setup, we can selectively measure the superconducting gap

on different sections of the electron pockets (Fig. 3). The gap anisotropy is obvious near the

major axis of the ellipses (Figs. 3a ~ 3f), and manifested by the maxima along the 90° and

270° directions in Figs. 3c and 3f, respectively.

Because the Fermi surface of 1ML FeSe is C4 symmetric, we could then map the gap

measurement data onto one ellipse electron pocket. The results are shown in Figs. 4a ~ 4b.

The smooth evolution of the gap tied to the underlying Fermi surface is consistent with it

being a superconducting gap. Because ARPES measures the absolute value of the gap

function we perform a best fit of the observed energy gap as a function of angle around the

Fermi pocket by |()| . The result of such fitting gives () = (9.98 ± 0.10) −

(1.24 ± 0.13) cos 2 + (1.15 ± 0.13) 4 meV.

One characteristic of the gap anisotropy is that the gap maxima locate along the major-axis of

the ellipse (the 90° and 270° directions). We simulated the gap distribution on the δ2 electron

pocket using several trigonometric gap functions that are proposed under d-wave, s± and

extended s-wave pairing symmetries (Figs. 4d ~ 4f). For the |(cos − cos) /2| and

| cos cos | gap functions, the pair strength is strongest at the center of the ellipse electron

pockets meaning that the gap maxima should locate along the minor-axis of the ellipse (0°

and 180° directions) (Figs. 4e and 4f). This contradicts to our observation. For the |(cos +

cos) /2| gap function, it generates gap maxima along the correct directions. However, the

|(cos + cos) /2| gap function is not energy favored in 1ML FeSe because the pairing

strength is strongest at the center and corner of the one-iron Brillouin zone where there is no

Fermi surface. In order to achieve the 8~13 meV gap magnitude on the electron pockets,

large and unrealistic gap value (> 100 meV) needs to be used in the simulation. Therefore, the

observed momentum locations of the gap maxima cannot be explained by a single

trigonometric gap function. Mixing of different gap functions with the same symmetry18 or

the high harmonic gap functions should be considered14. Alternatively, the gap anisotropy on

the δ2 ellipse electron pocket is C2 symmetric, which does not violate the crystal symmetry.

Therefore, the observed gap distribution can be consistent with an s-wave gap function if the

pairing strength varies on the Fermi surface following the crystal symmetry of material.

Another characteristic of the gap anisotropy is the presence of four gap minima along the 45°

directions of the ellipse. On one hand, the gap minima can be induced by the Fermi surface

hybridization near the intersection of the δ1 and δ2 ellipse electron pockets. According to the

band calculations, either the spin-orbital coupling or the breaking of glide-mirror symmetry

would lift the band degeneracy at the Fermi surface crossing of two ellipses in two-iron

Brillouin zone25, 26. For 1ML FeSe film grown on SrTiO3, finite spin-orbital coupling is

present as observed in bulk FeSe27 and the glide-mirror symmetry no longer exists due to the

presence of substrate. Therefore, it is expected that there is finite hybridization between the δ1

and δ2 ellipse electron pockets. If gap changes sign near the intersection of δ1 and δ2, such as

the gap under d-wave and extended s-wave pairing symmetries, the hybridization between δ1

and δ2 would mix the gaps with opposite sign and generate gap minima or gap nodes

depending on the strength of the hybridization13, 15. On the other hand, the gap minima may

originate from the multi-orbital nature of superconductivity. The electron pockets are

constructed by dxz/dyz and dxy orbitals and the orbital character varies when moving around the

Fermi surface20-23. The gap minima locate along the 45° directions of the ellipses where the

mixing of dxz/dyz and dxy orbitals is strongest. Gap would be minima if the intra-orbital pairing

dominates the pairing interaction in 1ML FeSe18.

Method

FeSe films were grown on high quality Nb-doped (0.05% wt) SrTiO3 (100) substrates. TiO2

terminated atomic flat surface were prepared by degassing at 450 °C for several hours and

subsequently annealing at 900 °C for 20 min. Ultrahigh purity selenium (99.999%) was

evaporated from an effusion cell with a thermal cracking insert (Createc) while iron

(99.995%) was evaporated from a 2 mm rod using an electron beam evaporator (Specs). The

growth was carried out under Se-rich condition with a Se/Fe flux ratio of 3~4. Substrate

temperatures were kept at 380 °C during the growth. The films were subsequently annealed at

450 °C for four hours immediately after growth. The films were transported to the Stanford

Synchrotron Radiation Lighsource Beamline 5-4 via a vacuum suitcase with base pressure of

5x10−10 Torr.

ARPES measurements were performed at the Stanford Synchrotron Radiation Lightsource

Beamline 5-4. The data were taken with 22 eV photons. The temperature was kept at 20 K for

the superconducting gap measurement. The overall energy resolution was 5 meV, and the

angular resolution was less than 0.3 degree. All the samples were measured in ultrahigh

vacuum with a base pressure better than 3×10−11 Torr.

References

FeSe Films on SrTiO3. Chin. Phys. Lett. 29, 37402-037402 (2012).

2. Liu, D. et al. Electronic origin of high-temperature superconductivity in single-layer FeSe

superconductor. Nat. Commun. 3, 931 (2012).

3. He, S. L. et al. Phase diagram and high temperature superconductivity at 65 K in tuning carrier

concentration of single-layer FeSe films. Nat. Mater. 12, 605–610 (2013).

4. Tan, S. et al. Interface-induced superconductivity and strain-dependent spin density waves in

FeSe/SrTiO3 thin films. Nat. Mater. 12, 634-640, (2013).

5. Zhang, W.-H. et al. Direct Observation of High-Temperature Superconductivity in One-Unit-

Cell FeSe Films. Chin. Phys. Lett. 31, 017401 (2014).

6. Peng, R. et al. Tuning the band structure and superconductivity in single-layer FeSe by interface

engineering. Nat. Commun. 5, 6044 (2014).

7. Deng, L. Z. et al. Meissner and mesoscopic superconducting states in 1-4 unit-cell FeSe films.

Phys. Rev. B 90, 214513 (2014).

8. Ge, J.-F. et al. Superconductivity in single-layer films of FeSe with a transition temperature

above 100 K. arXiv, 1406.3435 (2014).

9. Xiang, Y.-Y., Wang, F., Wang, D., Wang, Q.-H. & Lee, D.-H. High-temperature

superconductivity at the FeSe/SrTiO3 interface. Phys. Rev. B 86, 134508 (2012).

10. Lee, J. J. et al. Interfacial mode coupling as the origin of the enhancement of Tc in FeSe films on

SrTiO3. Nature 515, 245-248, (2014).

11. Coh, S., Cohen, M. L. & Louie, S. G. Structural template increases electron-phonon interaction

in an FeSe monolayer. arXiv, 1407.5657 (2014).

12. Timur, B. & Marvin, L. C. Effects of charge doping and constrained magnetization on the

electronic structure of an FeSe monolayer. Journal of Physics: Condensed Matter 25, 105506

(2013).

13. Hirschfeld, P. J., Korshunov, M. M. & Mazin, I. I. Gap symmetry and structure of Fe-based

superconductors. Rep. Prog. Phys. 74, 124508 (2011).

14. Maier, T. A., Graser, S., Hirschfeld, P. J. & Scalapino, D. J. d-wave pairing from spin

fluctuations in the KxFe2-ySe2 superconductors. Phys. Rev. B 83, 100515 (2011).

15. Mazin, I. I. Symmetry analysis of possible superconducting states in KxFe2-ySe2 superconductors.

Phys. Rev. B 84, 024529 (2011).

16. Hao, N. & Hu, J. Odd parity pairing and nodeless antiphase s± in iron-based superconductors.

Phys. Rev. B 89, 045144 (2014).

17. Yang, F., Wang, F. & Lee, D.-H. Fermiology, orbital order, orbital fluctuations, and Cooper

pairing in iron-based superconductors. Phys. Rev. B 88, 100504 (2013).

18. Saito, T., Onari, S. & Kontani, H. Emergence of fully gapped s++-wave and nodal d-wave states

mediated by orbital and spin fluctuations in a ten-orbital model of KFe2Se2. Phys. Rev. B 83,

140512 (2011).

19. Lin, C.-H., Chou, C.-P., Yin, W.-G. & Ku, W. Orbital-Parity Distinct Superconducting Pairing

Structures of Fe-based Superconductors under Glide Symmetry. arXiv, 1403.3687 (2014).

20. Kuroki, K. et al. Unconventional Pairing Originating from the Disconnected Fermi Surfaces of

Superconducting LaFeAsO1-xFx. Phys. Rev. Lett. 101, 087004 (2008).

21. Graser, S., Maier, T. A., Hirschfeld, P. J. & Scalapino, D. J. Near-degeneracy of several pairing

channels in multiorbital models for the Fe pnictides. New J. Phys. 11, 025016 (2009).

22. Brouet, V. et al. Impact of the two Fe unit cell on the electronic structure measured by ARPES

in iron pnictides. Phys. Rev. B 86, 075123 (2012).

23. Zhang, Y. et al. Orbital characters of bands in the iron-based superconductor BaFe1.85Co0.15As2.

Phys. Rev. B 83, 054510 (2011).

24. Norman, M. R., Randeria, M., Ding, H. & Campuzano, J. C. Phenomenology of the low-energy

spectral function in high-Tc superconductors. Phys. Rev. B 57, R11093-R11096 (1998).

25. Borisenko, S. et al. Direct observation of spin-orbit coupling in iron-based superconductor.

arXiv, 1409.8669 (2014).

26. Lin, C.-H. et al. One-Fe versus Two-Fe Brillouin Zone of Fe-Based Superconductors: Creation

of the Electron Pockets by Translational Symmetry Breaking. Phys. Rev. Lett. 107, 257001

(2011).

27. Zhang, P. et al. Observation of two distinct dxz/dyz band splittings in FeSe. Phys. Rev. B 91,

214503 (2015).

ARPES experiments were performed at the Stanford Synchrotron Radiation Lightsource,

which is operated by the Office of Basic Energy Sciences, U.S. Department of Energy. The

Stanford work is supported by the US DOE, Office of Basic Energy Science, Division of

Materials Science and Engineering. D.-H. L. was supported by the U.S. Department of

Energy, Office of Science, Basic Energy Sciences, Materials Sciences and Engineering

Division, grant DE-AC02-05CH11231.

Author Contributions

Y. Z. and Z. X. S conceived the project. Y. Z., J. J. L., R. G. M., W. L. and M. Y. took the

ARPES measurements. Y. Z. analyzed the data. W. L., J. J. L. and R. G. M. grew the films.

M. H. and D. H. L. assisted in ARPES measurements at Stanford Synchrotron Radiation

Lightsource. T. P. D. D. H. L. and Z.X. S supervised the project. Y. Z., D. H. L. and Z. X. S

wrote the paper with input from all coauthors.

Author Information

The authors declare no competing financial interests. Correspondence and request for

materials should be addressed to Z.-X. Shen ([email protected]).

Figure 1 | Fermi surface topology. a, Fermi surface mapping of 1ML FeSe taken in circular

(CR) polarization. The Brillouin zone is defined by the two-iron unit cell with the Γ-M

direction along the iron-iron bond direction. b, The one- and two- iron unit cells in the iron-

pnictogen/chalcogen plane (right panel) and the corresponding one- and two- iron Brillouin

zones and Fermi surfaces (left panel). c, Fermi surface mapping (left panel) and its second

derivative image (right panel) taken in CR polarization at ~120 K using high energy and

momentum resolution. The derivation was taken along both kx and ky direction. d is the same

as c, but taken with linear horizontal (LH) polarization. The in-plane polarization vector is

along the kx direction.

Figure 2 | Multi-gap behavior of the superconducting state. a, The second derivative

images of photoemission spectra taken in CR and linear vertical (LV) polarization at 20K.

The in-plane polarization vector is along the ky direction for LV polarization. The momenta of

cut #1 and cut #2 are shown in the inset of b. b, The corresponding MDCs taken at the Fermi

energy (EF) of the data in a. c, Symmetrized EDCs taken at the Fermi crossings (kF’s) of the

δ1 electron band with CR and LV polarization. The gap magnitude was obtained by fitting the

symmetrized EDCs (black dots) using a phenomenological superconducting spectra

function24. The fitting result is shown by the red solid line. d is the same as c but taken at the

kF’s of the δ2 electron band.

Figure 3 | Momentum dependence of the superconducting gaps on the electron pockets.

a, The Fermi surface mapping taken in LH polarization. The polarization vector is shown in

the inset. b, Symmetrized EDCs taken on one section of the electron pockets. The momenta

of the data points are shown in a. c, Merged image of the symmetrized EDCs in a, which

highlights the variation of the superconducting peak positions. d – k are the same as a and c,

but taken on different sections of the electron pockets.

Figure 4 | Superconducting gap anisotropy in 1ML FeSe. a and b, Superconducting gap

anisotropy on the ellipse-like electron pocket δ2. The gap magnitudes were obtained by fitting

the symmetrized EDCs in Fig.3 using a phenomenological superconducting spectral

function24. The gap measurement data were mapped onto δ2 ellipse pocket according to the

C4 rotational symmetry. The error bars are estimated by the fitting process. c,

Phenomenology function fitting of the gap anisotropy in 1ML FeSe. The residual values are

shown in the upper panel presenting the fitting quality. The fitting result is shown by the red

solid line with the function (9.98 ± 0.10) − (1.24 ± 0.13) cos 2 + (1.15 ± 0.13) cos 4

meV. d, Simulation of the gap anisotropy on the δ2 electron pocket using the |(cos −

cos) /2| gap function. The inset panel illustrates the sign change on the Fermi surface. e

and f are the same as d but calculated using | cos cos | and |(cos + cos) /2| gap

functions.

Y. Zhang1, 2, J. J. Lee1, 3, R. G. Moore1, W. Li1, M. Yi1, 3, M. Hashimoto4, D. H. Lu4, T. P.

Devereaux1, 3, D.-H. Lee5, 6 & Z.-X. Shen1, 3, *

1Stanford Institute for Materials and Energy Sciences, SLAC National Accelerator

Laboratory, 2575 Sand Hill Road, Menlo Park, California 94025, USA

2Advanced Light Source, Lawrence Berkeley National

Laboratory, Berkeley, California 94720, USA

3Geballe Laboratory for Advanced Materials, Departments of Physics and Applied Physics,

Stanford University, Stanford, California 94305, USA

4Stanford Synchrotron Radiation Lightsource, SLAC National Accelerator Laboratory,

2575 Sand Hill Road, Menlo Park, California 94025, USA

5Department of Physics, University of California at Berkeley, Berkeley, California, 94720,

USA

94720, USA

superconductor. Superconductivity in one monolayer (1ML) FeSe thin film has

attracted great interest recently due to its intriguing interfacial properties and possibly

high superconducting transition temperature (Tc) over 77 K1-12. Here, we report high-

resolution measurements of the Fermi surface and superconducting gaps in 1ML FeSe

using angle-resolved photoemission spectroscopy (ARPES). Two ellipse-like electron

pockets are clearly resolved overlapping with each other at the Brillouin zone corner.

The superconducting gap is nodeless but moderately anisotropic, which put strong

constraints on determining the pairing symmetry. The gap maxima locate along the

major axis of ellipse, which cannot be explained by a single d-wave, extended s-wave, or

s± gap function. Four gap minima are observed at the intersection of electron pockets

suggesting the existence of either a sign change or orbital-dependent pairing in 1ML

FeSe.

For 1ML FeSe thin film grown on SrTiO3, previous angle-resolved photoemission

spectroscopy (ARPES) studies showed that the Fermi surface consists only of electron

pockets at the corner of the Brillouin zone and there are no hole pockets at the zone center as

typically found in iron-based superconductors2-4, 10. Based on such a Fermi surface topology,

several pairing symmetries have been proposed theoretically13-19: d-wave and extended s-

wave pairing symmetries, where the gaps change sign between different parts of the Fermi

surface; s-wave and s± pairing symmetries, where there is no sign change on the Fermi

surface. In early studies, the superconducting gaps were found to be nearly isotropic on the

electron pockets2, 4, however they provide insufficient information to address the critical issue

of pairing symmetry in 1ML FeSe.

Here, we study the 1ML FeSe film using high-resolution ARPES. The film is grown on Nb-

doped SrTiO3 and the Tc is around 55K as reported in ref 10. As shown in Fig. 1a, the ARPES

intensity map shows one circular-like Fermi surface at M and no Fermi surface at the zone

center (Γ). This result is consistent with previous studies2-4, 10. However, by performing high-

resolution measurements at the M point using particular photon polarizations, two ellipse-like

electron pockets are clearly resolved (Figs. 1c and 1d). According to the band calculations,

the Fermi surface consists of one ellipse electron pocket at each Brillouin zone boundary in

one-iron Brillouin zone20, 21 (Fig. 1b). When the glide-mirror symmetry of the iron-selenium

plane is considered, the unit cell doubles and the Brillouin zone folds22. As a result, the

horizontal ellipse pocket (δ1) folds onto the vertical ellipse pocket (δ2) in the two-iron

Brillouin zone (Fig. 1b). This is consistent with the observed Fermi surface topology at the M

point (Figs. 1c and 1d). The photoemission intensity of the main band δ2, is much higher than

that of the folded band δ1 at the bottom corner of the two-iron Brillouin zone.

Clear delineation of Fermi surface is important for determining the gap structure in 1ML

FeSe. Figure 2 shows the superconducting gaps associated with the δ1 and δ2 electron bands

along the Γ-M direction. Two electron bands are clearly resolved in the second derivative

images along the M-Γ direction (Fig. 2a). The orbital selectivity of different polarizations

enables us to probe different bands separately22, 23, which is crucial for measuring the

superconducting gaps in a multi-band system. By using linear vertical polarization (LV), the

δ1 and δ2 bands can be probed selectively by choosing the cut momenta at either the left or

bottom corner of the Brillouin zone (Fig. 2b). The back bendings of bands are clearly

observed attesting for the high data quality. The gap magnitude is determined by the gap

fitting of symmetrized EDCs at the relevant kF’s (Figs. 2c and 2d), i.e., the gap minima of the

corresponding band dispersions (Fig. 2a). The superconducting gap is ~10 meV for the δ1

band and ~13 meV for the δ2 band.

The multi-gap behavior on δ1 and δ2 suggests that the superconducting gap is anisotropic. By

choosing different experimental setup, we can selectively measure the superconducting gap

on different sections of the electron pockets (Fig. 3). The gap anisotropy is obvious near the

major axis of the ellipses (Figs. 3a ~ 3f), and manifested by the maxima along the 90° and

270° directions in Figs. 3c and 3f, respectively.

Because the Fermi surface of 1ML FeSe is C4 symmetric, we could then map the gap

measurement data onto one ellipse electron pocket. The results are shown in Figs. 4a ~ 4b.

The smooth evolution of the gap tied to the underlying Fermi surface is consistent with it

being a superconducting gap. Because ARPES measures the absolute value of the gap

function we perform a best fit of the observed energy gap as a function of angle around the

Fermi pocket by |()| . The result of such fitting gives () = (9.98 ± 0.10) −

(1.24 ± 0.13) cos 2 + (1.15 ± 0.13) 4 meV.

One characteristic of the gap anisotropy is that the gap maxima locate along the major-axis of

the ellipse (the 90° and 270° directions). We simulated the gap distribution on the δ2 electron

pocket using several trigonometric gap functions that are proposed under d-wave, s± and

extended s-wave pairing symmetries (Figs. 4d ~ 4f). For the |(cos − cos) /2| and

| cos cos | gap functions, the pair strength is strongest at the center of the ellipse electron

pockets meaning that the gap maxima should locate along the minor-axis of the ellipse (0°

and 180° directions) (Figs. 4e and 4f). This contradicts to our observation. For the |(cos +

cos) /2| gap function, it generates gap maxima along the correct directions. However, the

|(cos + cos) /2| gap function is not energy favored in 1ML FeSe because the pairing

strength is strongest at the center and corner of the one-iron Brillouin zone where there is no

Fermi surface. In order to achieve the 8~13 meV gap magnitude on the electron pockets,

large and unrealistic gap value (> 100 meV) needs to be used in the simulation. Therefore, the

observed momentum locations of the gap maxima cannot be explained by a single

trigonometric gap function. Mixing of different gap functions with the same symmetry18 or

the high harmonic gap functions should be considered14. Alternatively, the gap anisotropy on

the δ2 ellipse electron pocket is C2 symmetric, which does not violate the crystal symmetry.

Therefore, the observed gap distribution can be consistent with an s-wave gap function if the

pairing strength varies on the Fermi surface following the crystal symmetry of material.

Another characteristic of the gap anisotropy is the presence of four gap minima along the 45°

directions of the ellipse. On one hand, the gap minima can be induced by the Fermi surface

hybridization near the intersection of the δ1 and δ2 ellipse electron pockets. According to the

band calculations, either the spin-orbital coupling or the breaking of glide-mirror symmetry

would lift the band degeneracy at the Fermi surface crossing of two ellipses in two-iron

Brillouin zone25, 26. For 1ML FeSe film grown on SrTiO3, finite spin-orbital coupling is

present as observed in bulk FeSe27 and the glide-mirror symmetry no longer exists due to the

presence of substrate. Therefore, it is expected that there is finite hybridization between the δ1

and δ2 ellipse electron pockets. If gap changes sign near the intersection of δ1 and δ2, such as

the gap under d-wave and extended s-wave pairing symmetries, the hybridization between δ1

and δ2 would mix the gaps with opposite sign and generate gap minima or gap nodes

depending on the strength of the hybridization13, 15. On the other hand, the gap minima may

originate from the multi-orbital nature of superconductivity. The electron pockets are

constructed by dxz/dyz and dxy orbitals and the orbital character varies when moving around the

Fermi surface20-23. The gap minima locate along the 45° directions of the ellipses where the

mixing of dxz/dyz and dxy orbitals is strongest. Gap would be minima if the intra-orbital pairing

dominates the pairing interaction in 1ML FeSe18.

Method

FeSe films were grown on high quality Nb-doped (0.05% wt) SrTiO3 (100) substrates. TiO2

terminated atomic flat surface were prepared by degassing at 450 °C for several hours and

subsequently annealing at 900 °C for 20 min. Ultrahigh purity selenium (99.999%) was

evaporated from an effusion cell with a thermal cracking insert (Createc) while iron

(99.995%) was evaporated from a 2 mm rod using an electron beam evaporator (Specs). The

growth was carried out under Se-rich condition with a Se/Fe flux ratio of 3~4. Substrate

temperatures were kept at 380 °C during the growth. The films were subsequently annealed at

450 °C for four hours immediately after growth. The films were transported to the Stanford

Synchrotron Radiation Lighsource Beamline 5-4 via a vacuum suitcase with base pressure of

5x10−10 Torr.

ARPES measurements were performed at the Stanford Synchrotron Radiation Lightsource

Beamline 5-4. The data were taken with 22 eV photons. The temperature was kept at 20 K for

the superconducting gap measurement. The overall energy resolution was 5 meV, and the

angular resolution was less than 0.3 degree. All the samples were measured in ultrahigh

vacuum with a base pressure better than 3×10−11 Torr.

References

FeSe Films on SrTiO3. Chin. Phys. Lett. 29, 37402-037402 (2012).

2. Liu, D. et al. Electronic origin of high-temperature superconductivity in single-layer FeSe

superconductor. Nat. Commun. 3, 931 (2012).

3. He, S. L. et al. Phase diagram and high temperature superconductivity at 65 K in tuning carrier

concentration of single-layer FeSe films. Nat. Mater. 12, 605–610 (2013).

4. Tan, S. et al. Interface-induced superconductivity and strain-dependent spin density waves in

FeSe/SrTiO3 thin films. Nat. Mater. 12, 634-640, (2013).

5. Zhang, W.-H. et al. Direct Observation of High-Temperature Superconductivity in One-Unit-

Cell FeSe Films. Chin. Phys. Lett. 31, 017401 (2014).

6. Peng, R. et al. Tuning the band structure and superconductivity in single-layer FeSe by interface

engineering. Nat. Commun. 5, 6044 (2014).

7. Deng, L. Z. et al. Meissner and mesoscopic superconducting states in 1-4 unit-cell FeSe films.

Phys. Rev. B 90, 214513 (2014).

8. Ge, J.-F. et al. Superconductivity in single-layer films of FeSe with a transition temperature

above 100 K. arXiv, 1406.3435 (2014).

9. Xiang, Y.-Y., Wang, F., Wang, D., Wang, Q.-H. & Lee, D.-H. High-temperature

superconductivity at the FeSe/SrTiO3 interface. Phys. Rev. B 86, 134508 (2012).

10. Lee, J. J. et al. Interfacial mode coupling as the origin of the enhancement of Tc in FeSe films on

SrTiO3. Nature 515, 245-248, (2014).

11. Coh, S., Cohen, M. L. & Louie, S. G. Structural template increases electron-phonon interaction

in an FeSe monolayer. arXiv, 1407.5657 (2014).

12. Timur, B. & Marvin, L. C. Effects of charge doping and constrained magnetization on the

electronic structure of an FeSe monolayer. Journal of Physics: Condensed Matter 25, 105506

(2013).

13. Hirschfeld, P. J., Korshunov, M. M. & Mazin, I. I. Gap symmetry and structure of Fe-based

superconductors. Rep. Prog. Phys. 74, 124508 (2011).

14. Maier, T. A., Graser, S., Hirschfeld, P. J. & Scalapino, D. J. d-wave pairing from spin

fluctuations in the KxFe2-ySe2 superconductors. Phys. Rev. B 83, 100515 (2011).

15. Mazin, I. I. Symmetry analysis of possible superconducting states in KxFe2-ySe2 superconductors.

Phys. Rev. B 84, 024529 (2011).

16. Hao, N. & Hu, J. Odd parity pairing and nodeless antiphase s± in iron-based superconductors.

Phys. Rev. B 89, 045144 (2014).

17. Yang, F., Wang, F. & Lee, D.-H. Fermiology, orbital order, orbital fluctuations, and Cooper

pairing in iron-based superconductors. Phys. Rev. B 88, 100504 (2013).

18. Saito, T., Onari, S. & Kontani, H. Emergence of fully gapped s++-wave and nodal d-wave states

mediated by orbital and spin fluctuations in a ten-orbital model of KFe2Se2. Phys. Rev. B 83,

140512 (2011).

19. Lin, C.-H., Chou, C.-P., Yin, W.-G. & Ku, W. Orbital-Parity Distinct Superconducting Pairing

Structures of Fe-based Superconductors under Glide Symmetry. arXiv, 1403.3687 (2014).

20. Kuroki, K. et al. Unconventional Pairing Originating from the Disconnected Fermi Surfaces of

Superconducting LaFeAsO1-xFx. Phys. Rev. Lett. 101, 087004 (2008).

21. Graser, S., Maier, T. A., Hirschfeld, P. J. & Scalapino, D. J. Near-degeneracy of several pairing

channels in multiorbital models for the Fe pnictides. New J. Phys. 11, 025016 (2009).

22. Brouet, V. et al. Impact of the two Fe unit cell on the electronic structure measured by ARPES

in iron pnictides. Phys. Rev. B 86, 075123 (2012).

23. Zhang, Y. et al. Orbital characters of bands in the iron-based superconductor BaFe1.85Co0.15As2.

Phys. Rev. B 83, 054510 (2011).

24. Norman, M. R., Randeria, M., Ding, H. & Campuzano, J. C. Phenomenology of the low-energy

spectral function in high-Tc superconductors. Phys. Rev. B 57, R11093-R11096 (1998).

25. Borisenko, S. et al. Direct observation of spin-orbit coupling in iron-based superconductor.

arXiv, 1409.8669 (2014).

26. Lin, C.-H. et al. One-Fe versus Two-Fe Brillouin Zone of Fe-Based Superconductors: Creation

of the Electron Pockets by Translational Symmetry Breaking. Phys. Rev. Lett. 107, 257001

(2011).

27. Zhang, P. et al. Observation of two distinct dxz/dyz band splittings in FeSe. Phys. Rev. B 91,

214503 (2015).

ARPES experiments were performed at the Stanford Synchrotron Radiation Lightsource,

which is operated by the Office of Basic Energy Sciences, U.S. Department of Energy. The

Stanford work is supported by the US DOE, Office of Basic Energy Science, Division of

Materials Science and Engineering. D.-H. L. was supported by the U.S. Department of

Energy, Office of Science, Basic Energy Sciences, Materials Sciences and Engineering

Division, grant DE-AC02-05CH11231.

Author Contributions

Y. Z. and Z. X. S conceived the project. Y. Z., J. J. L., R. G. M., W. L. and M. Y. took the

ARPES measurements. Y. Z. analyzed the data. W. L., J. J. L. and R. G. M. grew the films.

M. H. and D. H. L. assisted in ARPES measurements at Stanford Synchrotron Radiation

Lightsource. T. P. D. D. H. L. and Z.X. S supervised the project. Y. Z., D. H. L. and Z. X. S

wrote the paper with input from all coauthors.

Author Information

The authors declare no competing financial interests. Correspondence and request for

materials should be addressed to Z.-X. Shen ([email protected]).

Figure 1 | Fermi surface topology. a, Fermi surface mapping of 1ML FeSe taken in circular

(CR) polarization. The Brillouin zone is defined by the two-iron unit cell with the Γ-M

direction along the iron-iron bond direction. b, The one- and two- iron unit cells in the iron-

pnictogen/chalcogen plane (right panel) and the corresponding one- and two- iron Brillouin

zones and Fermi surfaces (left panel). c, Fermi surface mapping (left panel) and its second

derivative image (right panel) taken in CR polarization at ~120 K using high energy and

momentum resolution. The derivation was taken along both kx and ky direction. d is the same

as c, but taken with linear horizontal (LH) polarization. The in-plane polarization vector is

along the kx direction.

Figure 2 | Multi-gap behavior of the superconducting state. a, The second derivative

images of photoemission spectra taken in CR and linear vertical (LV) polarization at 20K.

The in-plane polarization vector is along the ky direction for LV polarization. The momenta of

cut #1 and cut #2 are shown in the inset of b. b, The corresponding MDCs taken at the Fermi

energy (EF) of the data in a. c, Symmetrized EDCs taken at the Fermi crossings (kF’s) of the

δ1 electron band with CR and LV polarization. The gap magnitude was obtained by fitting the

symmetrized EDCs (black dots) using a phenomenological superconducting spectra

function24. The fitting result is shown by the red solid line. d is the same as c but taken at the

kF’s of the δ2 electron band.

Figure 3 | Momentum dependence of the superconducting gaps on the electron pockets.

a, The Fermi surface mapping taken in LH polarization. The polarization vector is shown in

the inset. b, Symmetrized EDCs taken on one section of the electron pockets. The momenta

of the data points are shown in a. c, Merged image of the symmetrized EDCs in a, which

highlights the variation of the superconducting peak positions. d – k are the same as a and c,

but taken on different sections of the electron pockets.

Figure 4 | Superconducting gap anisotropy in 1ML FeSe. a and b, Superconducting gap

anisotropy on the ellipse-like electron pocket δ2. The gap magnitudes were obtained by fitting

the symmetrized EDCs in Fig.3 using a phenomenological superconducting spectral

function24. The gap measurement data were mapped onto δ2 ellipse pocket according to the

C4 rotational symmetry. The error bars are estimated by the fitting process. c,

Phenomenology function fitting of the gap anisotropy in 1ML FeSe. The residual values are

shown in the upper panel presenting the fitting quality. The fitting result is shown by the red

solid line with the function (9.98 ± 0.10) − (1.24 ± 0.13) cos 2 + (1.15 ± 0.13) cos 4

meV. d, Simulation of the gap anisotropy on the δ2 electron pocket using the |(cos −

cos) /2| gap function. The inset panel illustrates the sign change on the Fermi surface. e

and f are the same as d but calculated using | cos cos | and |(cos + cos) /2| gap

functions.